The material structure described by LiFe2(BO3)2 crystallizes in the monoclinic Pc space group. There are two inequivalent Li sites. In the first Li site, Li(1) is bonded in a 4-coordinate geometry to one O(1), one O(12), one O(2), and one O(3) atom. In the second Li site, Li(2) is bonded to one O(10), one O(3), one O(5), one O(7), and one O(9) atom to form distorted LiO5 trigonal bipyramids that share  a cornercorner with one Fe(4)O5 trigonal bipyramid, corners with two equivalent Fe(1)O5 trigonal bipyramids,  an edgeedge with one Fe(2)O5 trigonal bipyramid, and  an edgeedge with one Fe(3)O5 trigonal bipyramid. There are four inequivalent Fe sites. In the first Fe site, Fe(1) is bonded to one O(10), one O(2), one O(4), one O(5), and one O(6) atom to form distorted FeO5 trigonal bipyramids that share corners with two equivalent Li(2)O5 trigonal bipyramids and edges with two equivalent Fe(2)O5 trigonal bipyramids. In the second Fe site, Fe(2) is bonded to one O(2), one O(4), one O(5), one O(6), and one O(7) atom to form FeO5 trigonal bipyramids that share  an edgeedge with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(1)O5 trigonal bipyramids. In the third Fe site, Fe(3) is bonded to one O(11), one O(12), one O(3), one O(8), and one O(9) atom to form distorted FeO5 trigonal bipyramids that share  an edgeedge with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(4)O5 trigonal bipyramids. In the fourth Fe site, Fe(4) is bonded to one O(1), one O(11), one O(12), one O(8), and one O(9) atom to form FeO5 trigonal bipyramids that share  a cornercorner with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(3)O5 trigonal bipyramids. There are four inequivalent B sites. In the first B site, B(1) is bonded in a trigonal planar geometry to one O(1), one O(5), and one O(6) atom. In the second B site, B(2) is bonded in a trigonal planar geometry to one O(2), one O(3), and one O(4) atom. In the third B site, B(3) is bonded in a trigonal planar geometry to one O(11), one O(12), and one O(7) atom. In the fourth B site, B(4) is bonded in a trigonal planar geometry to one O(10), one O(8), and one O(9) atom. There are twelve inequivalent O sites. In the first O site, O(1) is bonded in a distorted trigonal non-coplanar geometry to one Li(1), one Fe(4), and one B(1) atom. In the second O site, O(2) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Fe(1), one Fe(2), and one B(2) atom. In the third O site, O(3) is bonded in a distorted trigonal pyramidal geometry to one Li(1), one Li(2), one Fe(3), and one B(2) atom. In the fourth O site, O(4) is bonded in a distorted trigonal planar geometry to one Fe(1), one Fe(2), and one B(2) atom. In the fifth O site, O(5) is bonded in a 4-coordinate geometry to one Li(2), one Fe(1), one Fe(2), and one B(1) atom. In the sixth O site, O(6) is bonded in a distorted trigonal planar geometry to one Fe(1), one Fe(2), and one B(1) atom. In the seventh O site, O(7) is bonded in a 3-coordinate geometry to one Li(2), one Fe(2), and one B(3) atom. In the eighth O site, O(8) is bonded in a 3-coordinate geometry to one Fe(3), one Fe(4), and one B(4) atom. In the ninth O site, O(9) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Fe(3), one Fe(4), and one B(4) atom. In the tenth O site, O(10) is bonded in a 3-coordinate geometry to one Li(2), one Fe(1), and one B(4) atom. In the eleventh O site, O(11) is bonded in a distorted trigonal planar geometry to one Fe(3), one Fe(4), and one B(3) atom. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Fe(3), one Fe(4), and one B(3) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_LiFe2(BO3)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   9.066
_cell_length_b   5.264
_cell_length_c   11.370
_cell_angle_alpha   64.157
_cell_angle_beta   90.000
_cell_angle_gamma   90.000
_symmetry_Int_Tables_number   1
_cell_volume   488.312
_cell_formula_units_Z   4
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.259  0.506  0.151  1.0
  Li  Li1  1  0.249  0.449  0.891  1.0
  Li  Li2  1  0.751  0.449  0.391  1.0
  Li  Li3  1  0.741  0.506  0.651  1.0
  Fe  Fe4  1  0.416  0.963  0.879  1.0
  Fe  Fe5  1  0.411  0.533  0.630  1.0
  Fe  Fe6  1  0.589  0.533  0.130  1.0
  Fe  Fe7  1  0.584  0.963  0.379  1.0
  Fe  Fe8  1  0.918  0.027  0.629  1.0
  Fe  Fe9  1  0.086  0.465  0.378  1.0
  Fe  Fe10  1  0.914  0.465  0.878  1.0
  Fe  Fe11  1  0.082  0.027  0.129  1.0
  B  B12  1  0.419  0.473  0.375  1.0
  B  B13  1  0.583  0.049  0.626  1.0
  B  B14  1  0.417  0.049  0.126  1.0
  B  B15  1  0.581  0.473  0.875  1.0
  B  B16  1  0.919  0.522  0.133  1.0
  B  B17  1  0.917  0.947  0.381  1.0
  B  B18  1  0.083  0.947  0.881  1.0
  B  B19  1  0.081  0.522  0.633  1.0
  O  O20  1  0.285  0.394  0.346  1.0
  O  O21  1  0.429  0.816  0.098  1.0
  O  O22  1  0.285  0.192  0.104  1.0
  O  O23  1  0.462  0.139  0.672  1.0
  O  O24  1  0.549  0.389  0.336  1.0
  O  O25  1  0.451  0.389  0.836  1.0
  O  O26  1  0.430  0.643  0.439  1.0
  O  O27  1  0.570  0.643  0.939  1.0
  O  O28  1  0.715  0.192  0.604  1.0
  O  O29  1  0.571  0.816  0.598  1.0
  O  O30  1  0.538  0.139  0.172  1.0
  O  O31  1  0.786  0.608  0.159  1.0
  O  O32  1  0.715  0.394  0.846  1.0
  O  O33  1  0.959  0.861  0.836  1.0
  O  O34  1  0.930  0.177  0.412  1.0
  O  O35  1  0.786  0.808  0.398  1.0
  O  O36  1  0.930  0.352  0.069  1.0
  O  O37  1  0.070  0.352  0.569  1.0
  O  O38  1  0.050  0.601  0.175  1.0
  O  O39  1  0.950  0.601  0.675  1.0
  O  O40  1  0.041  0.861  0.336  1.0
  O  O41  1  0.214  0.808  0.898  1.0
  O  O42  1  0.070  0.177  0.912  1.0
  O  O43  1  0.214  0.608  0.659  1.0
[/CIF]
.
The material structure described by LiFe2(BO3)2 crystallizes in the monoclinic Pc space group. There are two inequivalent Li sites. In the first Li site, Li(1) is bonded in a 4-coordinate geometry to one O(1), one O(12), one O(2), and one O(3) atom. In the second Li site, Li(2) is bonded to one O(10), one O(3), one O(5), one O(7), and one O(9) atom to form distorted LiO5 trigonal bipyramids that share  a cornercorner with one Fe(4)O5 trigonal bipyramid, corners with two equivalent Fe(1)O5 trigonal bipyramids,  an edgeedge with one Fe(2)O5 trigonal bipyramid, and  an edgeedge with one Fe(3)O5 trigonal bipyramid. There are four inequivalent Fe sites. In the first Fe site, Fe(1) is bonded to one O(10), one O(2), one O(4), one O(5), and one O(6) atom to form distorted FeO5 trigonal bipyramids that share corners with two equivalent Li(2)O5 trigonal bipyramids and edges with two equivalent Fe(2)O5 trigonal bipyramids. In the second Fe site, Fe(2) is bonded to one O(2), one O(4), one O(5), one O(6), and one O(7) atom to form FeO5 trigonal bipyramids that share  an edgeedge with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(1)O5 trigonal bipyramids. In the third Fe site, Fe(3) is bonded to one O(11), one O(12), one O(3), one O(8), and one O(9) atom to form distorted FeO5 trigonal bipyramids that share  an edgeedge with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(4)O5 trigonal bipyramids. In the fourth Fe site, Fe(4) is bonded to one O(1), one O(11), one O(12), one O(8), and one O(9) atom to form FeO5 trigonal bipyramids that share  a cornercorner with one Li(2)O5 trigonal bipyramid and edges with two equivalent Fe(3)O5 trigonal bipyramids. There are four inequivalent B sites. In the first B site, B(1) is bonded in a trigonal planar geometry to one O(1), one O(5), and one O(6) atom. In the second B site, B(2) is bonded in a trigonal planar geometry to one O(2), one O(3), and one O(4) atom. In the third B site, B(3) is bonded in a trigonal planar geometry to one O(11), one O(12), and one O(7) atom. In the fourth B site, B(4) is bonded in a trigonal planar geometry to one O(10), one O(8), and one O(9) atom. There are twelve inequivalent O sites. In the first O site, O(1) is bonded in a distorted trigonal non-coplanar geometry to one Li(1), one Fe(4), and one B(1) atom. In the second O site, O(2) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Fe(1), one Fe(2), and one B(2) atom. In the third O site, O(3) is bonded in a distorted trigonal pyramidal geometry to one Li(1), one Li(2), one Fe(3), and one B(2) atom. In the fourth O site, O(4) is bonded in a distorted trigonal planar geometry to one Fe(1), one Fe(2), and one B(2) atom. In the fifth O site, O(5) is bonded in a 4-coordinate geometry to one Li(2), one Fe(1), one Fe(2), and one B(1) atom. In the sixth O site, O(6) is bonded in a distorted trigonal planar geometry to one Fe(1), one Fe(2), and one B(1) atom. In the seventh O site, O(7) is bonded in a 3-coordinate geometry to one Li(2), one Fe(2), and one B(3) atom. In the eighth O site, O(8) is bonded in a 3-coordinate geometry to one Fe(3), one Fe(4), and one B(4) atom. In the ninth O site, O(9) is bonded in a distorted rectangular see-saw-like geometry to one Li(2), one Fe(3), one Fe(4), and one B(4) atom. In the tenth O site, O(10) is bonded in a 3-coordinate geometry to one Li(2), one Fe(1), and one B(4) atom. In the eleventh O site, O(11) is bonded in a distorted trigonal planar geometry to one Fe(3), one Fe(4), and one B(3) atom. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Fe(3), one Fe(4), and one B(3) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_LiFe2(BO3)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   9.066
_cell_length_b   5.264
_cell_length_c   11.370
_cell_angle_alpha   64.157
_cell_angle_beta   90.000
_cell_angle_gamma   90.000
_symmetry_Int_Tables_number   1
_cell_volume   488.312
_cell_formula_units_Z   4
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.259  0.506  0.151  1.0
  Li  Li1  1  0.249  0.449  0.891  1.0
  Li  Li2  1  0.751  0.449  0.391  1.0
  Li  Li3  1  0.741  0.506  0.651  1.0
  Fe  Fe4  1  0.416  0.963  0.879  1.0
  Fe  Fe5  1  0.411  0.533  0.630  1.0
  Fe  Fe6  1  0.589  0.533  0.130  1.0
  Fe  Fe7  1  0.584  0.963  0.379  1.0
  Fe  Fe8  1  0.918  0.027  0.629  1.0
  Fe  Fe9  1  0.086  0.465  0.378  1.0
  Fe  Fe10  1  0.914  0.465  0.878  1.0
  Fe  Fe11  1  0.082  0.027  0.129  1.0
  B  B12  1  0.419  0.473  0.375  1.0
  B  B13  1  0.583  0.049  0.626  1.0
  B  B14  1  0.417  0.049  0.126  1.0
  B  B15  1  0.581  0.473  0.875  1.0
  B  B16  1  0.919  0.522  0.133  1.0
  B  B17  1  0.917  0.947  0.381  1.0
  B  B18  1  0.083  0.947  0.881  1.0
  B  B19  1  0.081  0.522  0.633  1.0
  O  O20  1  0.285  0.394  0.346  1.0
  O  O21  1  0.429  0.816  0.098  1.0
  O  O22  1  0.285  0.192  0.104  1.0
  O  O23  1  0.462  0.139  0.672  1.0
  O  O24  1  0.549  0.389  0.336  1.0
  O  O25  1  0.451  0.389  0.836  1.0
  O  O26  1  0.430  0.643  0.439  1.0
  O  O27  1  0.570  0.643  0.939  1.0
  O  O28  1  0.715  0.192  0.604  1.0
  O  O29  1  0.571  0.816  0.598  1.0
  O  O30  1  0.538  0.139  0.172  1.0
  O  O31  1  0.786  0.608  0.159  1.0
  O  O32  1  0.715  0.394  0.846  1.0
  O  O33  1  0.959  0.861  0.836  1.0
  O  O34  1  0.930  0.177  0.412  1.0
  O  O35  1  0.786  0.808  0.398  1.0
  O  O36  1  0.930  0.352  0.069  1.0
  O  O37  1  0.070  0.352  0.569  1.0
  O  O38  1  0.050  0.601  0.175  1.0
  O  O39  1  0.950  0.601  0.675  1.0
  O  O40  1  0.041  0.861  0.336  1.0
  O  O41  1  0.214  0.808  0.898  1.0
  O  O42  1  0.070  0.177  0.912  1.0
  O  O43  1  0.214  0.608  0.659  1.0
[/CIF]
.